#------------------------------------------------------------------------------
#$Date: 2016-03-21 18:01:52 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178799 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/53/4105384.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4105384
loop_
_publ_author_name
'Ginger E. Sigmon'
'Jie Ling'
'Daniel K. Unruh'
'Laura Moore-Shay'
'Matthew Ward'
'Brittany Weaver'
'Peter C. Burns'
_publ_contact_author_address
;University of Notre Dame
Dept. of Civil Engineering and Geological Sciences
156 Fitzpatrick Hall
Notre Dame, IN 46556
;
_publ_contact_author_email       pburns@nd.edu
_publ_contact_author_name        'Peter C. Burns'
_publ_contact_author_phone       574-631-5380
_publ_section_title
;
 Uranyl-Peroxide Interactions Favor Nanocluster Self-Assembly
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              16648
_journal_page_last               16649
_journal_paper_doi               10.1021/ja907837u
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'K+, (UO2)2+, (O2)2-, (C2O4)2-, (H2O)'
_chemical_formula_sum            'C10 K10 O53 U5'
_chemical_formula_weight         2549.25
_chemical_name_systematic
;
 Potassium uranyl peroxide oxalate hydrate
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.2949(7)
_cell_length_b                   19.5235(14)
_cell_length_c                   27.0032(19)
_cell_measurement_temperature    273(2)
_cell_volume                     5427.4(7)
_computing_cell_refinement       'SMART-NT v5.0'
_computing_data_collection       'SMART-NT v5.0'
_computing_data_reduction        'SMART-NT v5.0'
_computing_molecular_graphics    'CrystalMaker v1.4'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker PLATFORM with a SMART CCD Detector'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0892
_diffrn_reflns_av_sigmaI/netI    0.0626
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_limit_l_min       -37
_diffrn_reflns_number            80796
_diffrn_reflns_theta_full        29.17
_diffrn_reflns_theta_max         29.17
_diffrn_reflns_theta_min         2.09
_exptl_absorpt_coefficient_mu    15.760
_exptl_absorpt_correction_T_max  0.1681
_exptl_absorpt_correction_T_min  0.0513
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.120
_exptl_crystal_description       blocky
_exptl_crystal_F_000             4536
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.075
_exptl_crystal_size_min          0.050
_refine_diff_density_max         2.896
_refine_diff_density_min         -2.548
_refine_diff_density_rms         0.247
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.950
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     371
_refine_ls_number_reflns         7523
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.950
_refine_ls_R_factor_all          0.0423
_refine_ls_R_factor_gt           0.0287
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0334P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0759
_refine_ls_wR_factor_ref         0.0787
_reflns_number_gt                5665
_reflns_number_total             7523
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja907837u_si_003_3.cif
_cod_data_source_block           5ring
_cod_database_code               4105384
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z'
'-x-1/2, y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
U1 U 0.61644(4) 0.2500 0.299590(13) 0.00946(8) Uani 1 2 d S
U2 U 0.50730(3) 0.071824(13) 0.378242(10) 0.01051(6) Uani 1 1 d .
U3 U 0.30809(3) 0.137901(13) 0.506114(9) 0.01084(7) Uani 1 1 d .
K1 K 0.3309(2) 0.2500 0.39245(8) 0.0168(5) Uani 1 2 d S
K2 K 0.12475(17) 0.04830(9) 0.38136(7) 0.0206(4) Uani 1 1 d .
K3 K 0.0000(2) 0.2500 0.44277(8) 0.0165(5) Uani 1 2 d S
K4 K 0.85445(19) 0.11605(9) 0.25245(7) 0.0257(4) Uani 1 1 d .
K5 K 0.67534(18) 0.08973(9) 0.52783(6) 0.0236(4) Uani 1 1 d .
K6 K 0.4831(4) 0.2500 0.61124(14) 0.0530(10) Uani 1 2 d S
K7 K 0.1844(6) -0.1661(3) 0.25963(19) 0.0668(16) Uani 0.50 1 d P
O1 O 0.6523(5) 0.0277(3) 0.39442(19) 0.0175(12) Uani 1 1 d .
O2 O 0.2742(7) 0.2500 0.5352(3) 0.0175(16) Uani 1 2 d S
O3 O 0.4307(5) 0.0608(2) 0.45961(18) 0.0140(11) Uani 1 1 d .
O4 O 0.7902(7) 0.2500 0.2935(3) 0.0145(15) Uani 1 2 d S
O5 O 0.2088(5) 0.1566(2) 0.45296(18) 0.0140(11) Uani 1 1 d .
O6 O 0.6279(5) 0.1339(2) 0.31999(17) 0.0123(10) Uani 1 1 d .
O7 O 0.6265(5) 0.1741(2) 0.36632(17) 0.0130(11) Uani 1 1 d .
O8 O 0.2103(5) 0.0267(2) 0.51179(18) 0.0148(11) Uani 1 1 d .
O9 O 0.4969(5) 0.0085(3) 0.30070(19) 0.0225(13) Uani 1 1 d .
O10 O 0.4421(7) 0.2500 0.3027(2) 0.0133(15) Uani 1 2 d S
O11 O 0.0630(5) -0.0775(3) 0.4208(2) 0.0212(12) Uani 1 1 d .
O12 O 0.3621(5) 0.1152(2) 0.35863(18) 0.0138(11) Uani 1 1 d .
O13 O 0.1138(5) 0.1354(2) 0.5542(2) 0.0195(12) Uani 1 1 d .
O14 O 0.5981(5) 0.1818(2) 0.22574(18) 0.0146(11) Uani 1 1 d .
O15 O -0.0612(5) 0.0410(3) 0.4527(2) 0.0191(12) Uani 1 1 d .
O16 O 0.4068(5) 0.1213(2) 0.55912(18) 0.0147(11) Uani 1 1 d .
O17 O 0.4933(5) 0.1292(2) 0.45467(18) 0.0147(11) Uani 1 1 d .
O18 O -0.1965(5) 0.1605(3) 0.4478(2) 0.0232(13) Uani 1 1 d .
O19 O 0.3799(5) -0.0305(3) 0.38205(19) 0.0195(12) Uani 1 1 d .
O20 O 0.3906(7) 0.2500 0.5018(3) 0.0180(17) Uani 1 2 d S
O21 O 0.5708(6) 0.1799(3) 0.14296(19) 0.0230(13) Uani 1 1 d .
O22 O 0.3554(8) -0.1372(3) 0.3531(3) 0.059(2) Uani 1 1 d .
O23 O 0.483(2) -0.1020(9) 0.2723(7) 0.031(2) Uiso 0.356(14) 1 d P
O23A O 0.4256(11) -0.0838(5) 0.2584(4) 0.031(2) Uiso 0.644(14) 1 d P
O24 O -0.0383(8) 0.2500 0.5471(3) 0.030(2) Uani 1 2 d S
O25 O 0.2079(11) -0.2500 0.3708(5) 0.063(3) Uani 1 2 d S
O26 O 0.8880(6) 0.0193(4) 0.3270(2) 0.0427(17) Uani 1 1 d .
O27 O 0.6827(10) 0.2500 0.5363(5) 0.062(3) Uani 1 2 d S
O28 O 0.2599(9) 0.1744(4) 0.6615(3) 0.0123(15) Uiso 0.535(7) 1 d P
O28A O 0.2917(10) 0.1024(5) 0.6570(4) 0.0123(15) Uiso 0.465(7) 1 d P
O29 O 0.0230(11) -0.1728(5) 0.3397(3) 0.095(3) Uani 1 1 d .
O30 O 0.6729(7) 0.0159(5) 0.2234(3) 0.079(3) Uani 1 1 d .
C1 C -0.0440(8) -0.0803(4) 0.4406(3) 0.0171(16) Uani 1 1 d .
C2 C -0.1099(8) -0.0156(4) 0.4625(3) 0.0158(16) Uani 1 1 d .
C3 C 0.5838(7) 0.2101(4) 0.1831(3) 0.0152(15) Uani 1 1 d .
C4 C 0.3889(9) -0.0767(4) 0.3485(4) 0.033(2) Uani 1 1 d .
C5 C 0.4466(11) -0.0519(5) 0.2984(4) 0.043(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 U1 O10 177.4(3) . .
O4 U1 O7 91.5(2) . 7_565
O10 U1 O7 90.5(2) . 7_565
O4 U1 O7 91.5(2) . .
O10 U1 O7 90.5(2) . .
O7 U1 O7 78.8(2) 7_565 .
O4 U1 O6 88.37(14) . 7_565
O10 U1 O6 92.26(13) . 7_565
O7 U1 O6 36.86(16) 7_565 7_565
O7 U1 O6 115.57(16) . 7_565
O4 U1 O6 88.37(14) . .
O10 U1 O6 92.26(13) . .
O7 U1 O6 115.57(16) 7_565 .
O7 U1 O6 36.86(16) . .
O6 U1 O6 152.1(2) 7_565 .
O4 U1 O14 90.1(2) . .
O10 U1 O14 87.7(2) . .
O7 U1 O14 173.97(16) 7_565 .
O7 U1 O14 106.98(16) . .
O6 U1 O14 137.45(16) 7_565 .
O6 U1 O14 70.27(16) . .
O4 U1 O14 90.1(2) . 7_565
O10 U1 O14 87.7(2) . 7_565
O7 U1 O14 106.98(16) 7_565 7_565
O7 U1 O14 173.97(16) . 7_565
O6 U1 O14 70.27(16) 7_565 7_565
O6 U1 O14 137.45(16) . 7_565
O14 U1 O14 67.2(2) . 7_565
O4 U1 K4 47.76(9) . 7_565
O10 U1 K4 131.23(9) . 7_565
O7 U1 K4 78.08(12) 7_565 7_565
O7 U1 K4 131.77(13) . 7_565
O6 U1 K4 51.62(12) 7_565 7_565
O6 U1 K4 135.55(13) . 7_565
O14 U1 K4 98.83(12) . 7_565
O14 U1 K4 52.58(13) 7_565 7_565
O4 U1 K4 47.76(9) . .
O10 U1 K4 131.23(9) . .
O7 U1 K4 131.77(13) 7_565 .
O7 U1 K4 78.08(12) . .
O6 U1 K4 135.55(13) 7_565 .
O6 U1 K4 51.62(12) . .
O14 U1 K4 52.58(13) . .
O14 U1 K4 98.83(12) 7_565 .
K4 U1 K4 86.89(6) 7_565 .
O4 U1 K1 144.8(2) . .
O10 U1 K1 37.8(2) . .
O7 U1 K1 62.15(13) 7_565 .
O7 U1 K1 62.15(12) . .
O6 U1 K1 83.41(12) 7_565 .
O6 U1 K1 83.41(12) . .
O14 U1 K1 118.59(12) . .
O14 U1 K1 118.59(12) 7_565 .
K4 U1 K1 135.02(3) 7_565 .
K4 U1 K1 135.02(3) . .
O4 U1 K4 129.60(12) . 6_556
O10 U1 K4 49.04(11) . 6_556
O7 U1 K4 135.54(13) 7_565 6_556
O7 U1 K4 83.47(12) . 6_556
O6 U1 K4 138.52(13) 7_565 6_556
O6 U1 K4 58.92(12) . 6_556
O14 U1 K4 45.25(12) . 6_556
O14 U1 K4 91.01(12) 7_565 6_556
K4 U1 K4 139.845(17) 7_565 6_556
K4 U1 K4 82.40(3) . 6_556
K1 U1 K4 73.49(4) . 6_556
O1 U2 O12 177.1(2) . .
O1 U2 O6 88.3(2) . .
O12 U2 O6 89.9(2) . .
O1 U2 O3 90.4(2) . .
O12 U2 O3 92.3(2) . .
O6 U2 O3 148.80(16) . .
O1 U2 O17 93.8(2) . .
O12 U2 O17 89.0(2) . .
O6 U2 O17 112.07(16) . .
O3 U2 O17 36.94(16) . .
O1 U2 O7 90.4(2) . .
O12 U2 O7 89.6(2) . .
O6 U2 O7 36.57(16) . .
O3 U2 O7 112.30(16) . .
O17 U2 O7 75.50(16) . .
O1 U2 O19 92.6(2) . .
O12 U2 O19 87.2(2) . .
O6 U2 O19 138.74(17) . .
O3 U2 O19 72.46(17) . .
O17 U2 O19 109.03(17) . .
O7 U2 O19 174.37(17) . .
O1 U2 O9 90.1(2) . .
O12 U2 O9 87.1(2) . .
O6 U2 O9 73.04(17) . .
O3 U2 O9 138.15(17) . .
O17 U2 O9 173.61(18) . .
O7 U2 O9 109.54(17) . .
O19 U2 O9 65.71(18) . .
O1 U2 K1 142.21(17) . .
O12 U2 K1 39.65(16) . .
O6 U2 K1 81.55(12) . .
O3 U2 K1 80.49(12) . .
O17 U2 K1 57.76(12) . .
O7 U2 K1 60.48(12) . .
O19 U2 K1 118.70(13) . .
O9 U2 K1 120.76(14) . .
O1 U2 K4 131.17(17) . 6_556
O12 U2 K4 45.92(16) . 6_556
O6 U2 K4 59.94(12) . 6_556
O3 U2 K4 136.20(13) . 6_556
O17 U2 K4 130.84(12) . 6_556
O7 U2 K4 84.30(12) . 6_556
O19 U2 K4 90.15(13) . 6_556
O9 U2 K4 47.65(13) . 6_556
K1 U2 K4 73.22(4) . 6_556
O1 U2 K2 140.57(16) . .
O12 U2 K2 40.11(16) . .
O6 U2 K2 126.91(12) . .
O3 U2 K2 68.62(13) . .
O17 U2 K2 88.60(12) . .
O7 U2 K2 128.00(12) . .
O19 U2 K2 50.05(13) . .
O9 U2 K2 85.16(13) . .
K1 U2 K2 69.07(4) . .
K4 U2 K2 69.48(4) 6_556 .
O1 U2 K5 58.92(17) . .
O12 U2 K5 123.97(16) . .
O6 U2 K5 111.50(12) . .
O3 U2 K5 43.98(13) . .
O17 U2 K5 35.15(12) . .
O7 U2 K5 81.62(12) . .
O19 U2 K5 104.00(13) . .
O9 U2 K5 147.77(14) . .
K1 U2 K5 91.24(4) . .
K4 U2 K5 162.83(4) 6_556 .
K2 U2 K5 112.30(4) . .
O16 U3 O5 178.8(2) . .
O16 U3 O3 90.3(2) . .
O5 U3 O3 90.5(2) . .
O16 U3 O20 90.2(2) . .
O5 U3 O20 88.7(2) . .
O3 U3 O20 112.3(2) . .
O16 U3 O2 89.2(2) . .
O5 U3 O2 89.6(2) . .
O3 U3 O2 149.5(2) . .
O20 U3 O2 37.2(2) . .
O16 U3 O17 89.9(2) . .
O5 U3 O17 90.2(2) . .
O3 U3 O17 36.93(16) . .
O20 U3 O17 75.3(2) . .
O2 U3 O17 112.5(2) . .
O16 U3 O13 92.1(2) . .
O5 U3 O13 87.8(2) . .
O3 U3 O13 137.23(17) . .
O20 U3 O13 110.4(2) . .
O2 U3 O13 73.3(2) . .
O17 U3 O13 173.86(16) . .
O16 U3 O8 91.32(19) . .
O5 U3 O8 89.8(2) . .
O3 U3 O8 71.17(17) . .
O20 U3 O8 176.3(2) . .
O2 U3 O8 139.4(2) . .
O17 U3 O8 108.09(16) . .
O13 U3 O8 66.09(16) . .
O16 U3 K1 136.18(16) . .
O5 U3 K1 43.09(16) . .
O3 U3 K1 84.41(12) . .
O20 U3 K1 52.98(18) . .
O2 U3 K1 75.03(16) . .
O17 U3 K1 60.94(12) . .
O13 U3 K1 120.43(13) . .
O8 U3 K1 127.06(12) . .
O16 U3 K5 44.84(16) . .
O5 U3 K5 135.42(16) . .
O3 U3 K5 53.59(13) . .
O20 U3 K5 83.26(18) . .
O2 U3 K5 108.34(19) . .
O17 U3 K5 45.30(12) . .
O13 U3 K5 135.95(13) . .
O8 U3 K5 100.21(12) . .
K1 U3 K5 101.51(5) . .
O16 U3 K6 43.64(16) . .
O5 U3 K6 135.14(16) . .
O3 U3 K6 119.34(14) . .
O20 U3 K6 50.55(18) . .
O2 U3 K6 47.34(19) . .
O17 U3 K6 95.33(13) . .
O13 U3 K6 90.15(14) . .
O8 U3 K6 129.59(12) . .
K1 U3 K6 103.35(5) . .
K5 U3 K6 66.04(6) . .
O16 U3 K3 148.00(16) . .
O5 U3 K3 31.10(16) . .
O3 U3 K3 121.59(13) . .
O20 U3 K3 76.62(18) . .
O2 U3 K3 62.67(19) . .
O17 U3 K3 113.93(12) . .
O13 U3 K3 66.47(13) . .
O8 U3 K3 100.38(12) . .
K1 U3 K3 54.29(5) . .
K5 U3 K3 154.98(4) . .
K6 U3 K3 109.98(4) . .
O10 K1 O5 137.04(11) . .
O10 K1 O5 137.04(11) . 7_565
O5 K1 O5 83.0(2) . 7_565
O10 K1 O12 69.92(11) . 7_565
O5 K1 O12 150.15(16) . 7_565
O5 K1 O12 67.91(14) 7_565 7_565
O10 K1 O12 69.92(11) . .
O5 K1 O12 67.91(14) . .
O5 K1 O12 150.15(16) 7_565 .
O12 K1 O12 139.6(2) 7_565 .
O10 K1 O20 143.0(2) . .
O5 K1 O20 60.78(14) . .
O5 K1 O20 60.78(14) 7_565 .
O12 K1 O20 107.19(11) 7_565 .
O12 K1 O20 107.19(11) . .
O10 K1 O21 95.05(18) . 6_556
O5 K1 O21 60.33(14) . 6_556
O5 K1 O21 94.55(16) 7_565 6_556
O12 K1 O21 113.90(15) 7_565 6_556
O12 K1 O21 65.89(15) . 6_556
O20 K1 O21 118.00(17) . 6_556
O10 K1 O21 95.05(18) . 4_455
O5 K1 O21 94.55(16) . 4_455
O5 K1 O21 60.33(14) 7_565 4_455
O12 K1 O21 65.89(14) 7_565 4_455
O12 K1 O21 113.90(15) . 4_455
O20 K1 O21 118.00(17) . 4_455
O21 K1 O21 51.38(19) 6_556 4_455
O10 K1 O17 103.95(15) . 7_565
O5 K1 O17 113.42(15) . 7_565
O5 K1 O17 57.50(13) 7_565 7_565
O12 K1 O17 56.25(13) 7_565 7_565
O12 K1 O17 140.23(15) . 7_565
O20 K1 O17 53.58(11) . 7_565
O21 K1 O17 151.92(14) 6_556 7_565
O21 K1 O17 105.70(12) 4_455 7_565
O10 K1 O17 103.95(14) . .
O5 K1 O17 57.50(13) . .
O5 K1 O17 113.42(15) 7_565 .
O12 K1 O17 140.23(15) 7_565 .
O12 K1 O17 56.25(13) . .
O20 K1 O17 53.58(11) . .
O21 K1 O17 105.70(13) 6_556 .
O21 K1 O17 151.92(15) 4_455 .
O17 K1 O17 89.74(17) 7_565 .
O10 K1 C3 76.9(2) . 6_556
O5 K1 C3 81.99(17) . 6_556
O5 K1 C3 99.68(17) 7_565 6_556
O12 K1 C3 96.11(17) 7_565 6_556
O12 K1 C3 70.78(16) . 6_556
O20 K1 C3 138.6(2) . 6_556
O21 K1 C3 21.71(15) 6_556 6_556
O21 K1 C3 43.30(16) 4_455 6_556
O17 K1 C3 148.08(15) 7_565 6_556
O17 K1 C3 121.41(15) . 6_556
O10 K1 C3 76.9(2) . 4_455
O5 K1 C3 99.68(17) . 4_455
O5 K1 C3 81.99(17) 7_565 4_455
O12 K1 C3 70.78(16) 7_565 4_455
O12 K1 C3 96.11(17) . 4_455
O20 K1 C3 138.6(2) . 4_455
O21 K1 C3 43.30(16) 6_556 4_455
O21 K1 C3 21.71(15) 4_455 4_455
O17 K1 C3 121.41(15) 7_565 4_455
O17 K1 C3 148.08(15) . 4_455
C3 K1 C3 26.8(2) 6_556 4_455
O21 K2 O15 94.40(17) 6_556 .
O21 K2 O11 153.26(18) 6_556 .
O15 K2 O11 61.12(16) . .
O21 K2 O12 71.78(17) 6_556 .
O15 K2 O12 141.57(17) . .
O11 K2 O12 133.92(17) . .
O21 K2 O26 83.71(19) 6_556 1_455
O15 K2 O26 75.93(18) . 1_455
O11 K2 O26 80.07(18) . 1_455
O12 K2 O26 134.71(17) . 1_455
O21 K2 O30 90.3(2) 6_556 6_556
O15 K2 O30 142.08(19) . 6_556
O11 K2 O30 102.7(2) . 6_556
O12 K2 O30 75.27(18) . 6_556
O26 K2 O30 67.2(2) 1_455 6_556
O21 K2 O5 62.98(15) 6_556 .
O15 K2 O5 77.46(15) . .
O11 K2 O5 116.59(16) . .
O12 K2 O5 64.25(14) . .
O26 K2 O5 135.05(18) 1_455 .
O30 K2 O5 136.4(2) 6_556 .
O21 K2 O19 131.10(17) 6_556 .
O15 K2 O19 125.24(16) . .
O11 K2 O19 75.28(15) . .
O12 K2 O19 59.40(14) . .
O26 K2 O19 129.00(19) 1_455 .
O30 K2 O19 75.6(2) 6_556 .
O5 K2 O19 95.94(15) . .
O21 K2 C1 134.44(19) 6_556 .
O15 K2 C1 43.84(17) . .
O11 K2 C1 18.86(16) . .
O12 K2 C1 150.42(17) . .
O26 K2 C1 70.69(18) 1_455 .
O30 K2 C1 112.0(2) 6_556 .
O5 K2 C1 111.14(17) . .
O19 K2 C1 93.67(16) . .
O21 K2 C2 110.45(18) 6_556 .
O15 K2 C2 18.19(16) . .
O11 K2 C2 43.81(16) . .
O12 K2 C2 153.62(17) . .
O26 K2 C2 70.54(18) 1_455 .
O30 K2 C2 130.0(2) 6_556 .
O5 K2 C2 92.70(16) . .
O19 K2 C2 114.36(16) . .
C1 K2 C2 25.82(17) . .
O21 K2 U2 95.07(14) 6_556 .
O15 K2 U2 136.08(13) . .
O11 K2 U2 109.94(13) . .
O12 K2 U2 24.10(10) . .
O26 K2 U2 147.78(15) 1_455 .
O30 K2 U2 80.61(14) 6_556 .
O5 K2 U2 69.20(10) . .
O19 K2 U2 37.03(10) . .
C1 K2 U2 126.49(14) . .
C2 K2 U2 137.88(13) . .
O21 K2 K5 148.59(14) 6_556 5_656
O15 K2 K5 84.13(12) . 5_656
O11 K2 K5 46.53(12) . 5_656
O12 K2 K5 89.99(11) . 5_656
O26 K2 K5 125.74(15) 1_455 5_656
O30 K2 K5 110.0(2) 6_556 5_656
O5 K2 K5 86.23(10) . 5_656
O19 K2 K5 41.12(10) . 5_656
C1 K2 K5 60.45(13) . 5_656
C2 K2 K5 75.07(12) . 5_656
U2 K2 K5 66.34(4) . 5_656
O18 K3 O18 81.5(2) . 7_565
O18 K3 O21 85.39(18) . 6_556
O18 K3 O21 124.11(19) 7_565 6_556
O18 K3 O21 124.11(19) . 4_455
O18 K3 O21 85.39(18) 7_565 4_455
O21 K3 O21 58.8(2) 6_556 4_455
O18 K3 O5 171.47(18) . 7_565
O18 K3 O5 98.51(16) 7_565 7_565
O21 K3 O5 101.45(17) 6_556 7_565
O21 K3 O5 64.28(16) 4_455 7_565
O18 K3 O5 98.51(15) . .
O18 K3 O5 171.47(18) 7_565 .
O21 K3 O5 64.28(15) 6_556 .
O21 K3 O5 101.45(17) 4_455 .
O5 K3 O5 80.2(2) 7_565 .
O18 K3 O24 81.05(18) . .
O18 K3 O24 81.05(18) 7_565 .
O21 K3 O24 149.23(12) 6_556 .
O21 K3 O24 149.23(12) 4_455 .
O5 K3 O24 90.52(17) 7_565 .
O5 K3 O24 90.52(17) . .
O18 K3 K1 136.12(13) . .
O18 K3 K1 136.12(13) 7_565 .
O21 K3 K1 56.57(14) 6_556 .
O21 K3 K1 56.57(14) 4_455 .
O5 K3 K1 48.02(11) 7_565 .
O5 K3 K1 48.02(11) . .
O24 K3 K1 119.72(19) . .
O18 K3 U3 152.45(14) . 7_565
O18 K3 U3 102.04(12) 7_565 7_565
O21 K3 U3 113.28(14) 6_556 7_565
O21 K3 U3 83.42(12) 4_455 7_565
O5 K3 U3 19.16(10) 7_565 7_565
O5 K3 U3 73.98(11) . 7_565
O24 K3 U3 72.69(15) . 7_565
K1 K3 U3 56.74(4) . 7_565
O18 K3 U3 102.04(12) . .
O18 K3 U3 152.45(14) 7_565 .
O21 K3 U3 83.42(12) 6_556 .
O21 K3 U3 113.28(14) 4_455 .
O5 K3 U3 73.98(11) 7_565 .
O5 K3 U3 19.16(10) . .
O24 K3 U3 72.69(15) . .
K1 K3 U3 56.74(4) . .
U3 K3 U3 62.55(3) 7_565 .
O18 K3 K2 70.13(12) . .
O18 K3 K2 144.37(14) 7_565 .
O21 K3 K2 35.17(11) 6_556 .
O21 K3 K2 92.82(12) 4_455 .
O5 K3 K2 112.72(12) 7_565 .
O5 K3 K2 41.35(10) . .
O24 K3 K2 114.08(6) . .
K1 K3 K2 66.11(4) . .
U3 K3 K2 113.11(5) 7_565 .
U3 K3 K2 58.41(3) . .
O18 K3 K2 144.37(14) . 7_565
O18 K3 K2 70.13(12) 7_565 7_565
O21 K3 K2 92.82(12) 6_556 7_565
O21 K3 K2 35.17(11) 4_455 7_565
O5 K3 K2 41.35(10) 7_565 7_565
O5 K3 K2 112.72(12) . 7_565
O24 K3 K2 114.08(6) . 7_565
K1 K3 K2 66.11(4) . 7_565
U3 K3 K2 58.41(3) 7_565 7_565
U3 K3 K2 113.11(5) . 7_565
K2 K3 K2 123.93(7) . 7_565
O26 K4 O30 79.2(2) . .
O26 K4 O14 92.67(17) . 6_656
O30 K4 O14 160.9(2) . 6_656
O26 K4 O4 111.2(2) . .
O30 K4 O4 125.3(2) . .
O14 K4 O4 73.74(17) 6_656 .
O26 K4 O9 78.80(18) . 6_656
O30 K4 O9 72.5(2) . 6_656
O14 K4 O9 89.07(15) 6_656 6_656
O4 K4 O9 160.12(18) . 6_656
O26 K4 O6 74.58(17) . .
O30 K4 O6 74.48(18) . .
O14 K4 O6 120.30(15) 6_656 .
O4 K4 O6 59.03(16) . .
O9 K4 O6 140.66(15) 6_656 .
O26 K4 O12 135.74(18) . 6_656
O30 K4 O12 74.63(18) . 6_656
O14 K4 O12 100.60(15) 6_656 6_656
O4 K4 O12 112.99(17) . 6_656
O9 K4 O12 59.62(14) 6_656 6_656
O6 K4 O12 129.25(15) . 6_656
O26 K4 O14 124.74(17) . .
O30 K4 O14 69.5(2) . .
O14 K4 O14 128.33(18) 6_656 .
O4 K4 O14 60.76(17) . .
O9 K4 O14 128.56(15) 6_656 .
O6 K4 O14 54.07(13) . .
O12 K4 O14 77.68(14) 6_656 .
O26 K4 O10 150.7(2) . 6_656
O30 K4 O10 129.5(2) . 6_656
O14 K4 O10 58.36(16) 6_656 6_656
O4 K4 O10 59.91(16) . 6_656
O9 K4 O10 102.73(15) 6_656 6_656
O6 K4 O10 114.66(15) . 6_656
O12 K4 O10 61.53(15) 6_656 6_656
O14 K4 O10 77.52(16) . 6_656
O26 K4 C3 84.94(19) . 6_656
O30 K4 C3 164.0(2) . 6_656
O14 K4 C3 20.93(15) 6_656 6_656
O4 K4 C3 59.19(18) . 6_656
O9 K4 C3 106.54(17) 6_656 6_656
O6 K4 C3 99.44(16) . 6_656
O12 K4 C3 119.19(17) 6_656 6_656
O14 K4 C3 119.36(16) . 6_656
O10 K4 C3 66.46(18) 6_656 6_656
O26 K4 U1 107.76(15) . .
O30 K4 U1 98.2(2) . .
O14 K4 U1 100.73(11) 6_656 .
O4 K4 U1 27.13(13) . .
O9 K4 U1 167.75(12) 6_656 .
O6 K4 U1 37.90(9) . .
O12 K4 U1 110.80(11) 6_656 .
O14 K4 U1 39.21(9) . .
O10 K4 U1 76.77(11) 6_656 .
C3 K4 U1 84.62(12) 6_656 .
O26 K4 U2 116.56(16) . 6_656
O30 K4 U2 82.18(15) . 6_656
O14 K4 U2 86.17(11) 6_656 6_656
O4 K4 U2 128.64(13) . 6_656
O9 K4 U2 37.79(10) 6_656 6_656
O6 K4 U2 151.85(11) . 6_656
O12 K4 U2 25.50(10) 6_656 6_656
O14 K4 U2 103.12(10) . 6_656
O10 K4 U2 69.22(11) 6_656 6_656
C3 K4 U2 107.03(13) 6_656 6_656
U1 K4 U2 134.78(5) . 6_656
O19 K5 O8 94.83(16) 5_656 5_656
O19 K5 O17 126.46(17) 5_656 .
O8 K5 O17 103.57(15) 5_656 .
O19 K5 O18 163.28(17) 5_656 1_655
O8 K5 O18 84.80(15) 5_656 1_655
O17 K5 O18 69.50(15) . 1_655
O19 K5 O16 69.00(15) 5_656 .
O8 K5 O16 132.66(16) 5_656 .
O17 K5 O16 61.54(14) . .
O18 K5 O16 122.85(15) 1_655 .
O19 K5 O11 75.33(15) 5_656 5_656
O8 K5 O11 74.69(15) 5_656 5_656
O17 K5 O11 157.97(16) . 5_656
O18 K5 O11 88.51(16) 1_655 5_656
O16 K5 O11 135.62(15) . 5_656
O19 K5 O27 111.0(3) 5_656 .
O8 K5 O27 146.6(2) 5_656 .
O17 K5 O27 78.2(2) . .
O18 K5 O27 64.3(2) 1_655 .
O16 K5 O27 78.1(2) . .
O11 K5 O27 91.3(2) 5_656 .
O19 K5 O3 56.08(15) 5_656 5_656
O8 K5 O3 54.88(14) 5_656 5_656
O17 K5 O3 95.70(14) . 5_656
O18 K5 O3 133.26(15) 1_655 5_656
O16 K5 O3 80.77(14) . 5_656
O11 K5 O3 100.65(14) 5_656 5_656
O27 K5 O3 158.4(2) . 5_656
O19 K5 O3 105.93(15) 5_656 .
O8 K5 O3 88.11(14) 5_656 .
O17 K5 O3 27.98(12) . .
O18 K5 O3 90.78(15) 1_655 .
O16 K5 O3 57.33(13) . .
O11 K5 O3 162.78(14) 5_656 .
O27 K5 O3 103.8(2) . .
O3 K5 O3 67.76(15) 5_656 .
O19 K5 O22 41.50(16) 5_656 5_656
O8 K5 O22 129.40(18) 5_656 5_656
O17 K5 O22 122.03(19) . 5_656
O18 K5 O22 128.87(17) 1_655 5_656
O16 K5 O22 65.23(18) . 5_656
O11 K5 O22 70.63(18) 5_656 5_656
O27 K5 O22 70.0(2) . 5_656
O3 K5 O22 96.98(15) 5_656 5_656
O3 K5 O22 122.01(18) . 5_656
O19 K5 C4 20.65(17) 5_656 5_656
O8 K5 C4 113.47(18) 5_656 5_656
O17 K5 C4 125.10(19) . 5_656
O18 K5 C4 149.00(19) 1_655 5_656
O16 K5 C4 63.56(19) . 5_656
O11 K5 C4 73.69(19) 5_656 5_656
O27 K5 C4 90.4(3) . 5_656
O3 K5 C4 76.01(17) 5_656 5_656
O3 K5 C4 113.66(18) . 5_656
O22 K5 C4 21.02(17) 5_656 5_656
O19 K5 C2 109.24(17) 5_656 1_655
O8 K5 C2 19.17(15) 5_656 1_655
O17 K5 C2 103.09(16) . 1_655
O18 K5 C2 67.31(16) 1_655 1_655
O16 K5 C2 149.09(17) . 1_655
O11 K5 C2 67.92(16) 5_656 1_655
O27 K5 C2 127.4(2) . 1_655
O3 K5 C2 74.04(16) 5_656 1_655
O3 K5 C2 95.99(16) . 1_655
O22 K5 C2 134.8(2) 5_656 1_655
C4 K5 C2 124.90(19) 5_656 1_655
O27 K6 O22 80.0(2) . 3_656
O27 K6 O22 80.0(2) . 5_656
O22 K6 O22 97.8(3) 3_656 5_656
O27 K6 O2 91.8(3) . .
O22 K6 O2 129.70(16) 3_656 .
O22 K6 O2 129.70(16) 5_656 .
O27 K6 O16 81.77(18) . .
O22 K6 O16 159.9(2) 3_656 .
O22 K6 O16 70.76(18) 5_656 .
O2 K6 O16 58.95(12) . .
O27 K6 O16 81.77(17) . 7_565
O22 K6 O16 70.76(17) 3_656 7_565
O22 K6 O16 159.9(2) 5_656 7_565
O2 K6 O16 58.95(12) . 7_565
O16 K6 O16 114.7(2) . 7_565
O27 K6 O28 148.1(2) . 7_565
O22 K6 O28 85.3(2) 3_656 7_565
O22 K6 O28 130.3(3) 5_656 7_565
O2 K6 O28 76.2(2) . 7_565
O16 K6 O28 114.8(2) . 7_565
O16 K6 O28 66.7(2) 7_565 7_565
O27 K6 O28 148.1(2) . .
O22 K6 O28 130.3(3) 3_656 .
O22 K6 O28 85.3(2) 5_656 .
O2 K6 O28 76.2(2) . .
O16 K6 O28 66.7(2) . .
O16 K6 O28 114.8(2) 7_565 .
O28 K6 O28 57.9(3) 7_565 .
O27 K6 O20 63.3(3) . .
O22 K6 O20 119.20(19) 3_656 .
O22 K6 O20 119.20(19) 5_656 .
O2 K6 O20 28.47(19) . .
O16 K6 O20 58.04(11) . .
O16 K6 O20 58.04(11) 7_565 .
O28 K6 O20 101.1(2) 7_565 .
O28 K6 O20 101.1(2) . .
O27 K6 O25 53.2(3) . 5_656
O22 K6 O25 52.26(17) 3_656 5_656
O22 K6 O25 52.26(17) 5_656 5_656
O2 K6 O25 145.0(3) . 5_656
O16 K6 O25 109.34(16) . 5_656
O16 K6 O25 109.34(17) 7_565 5_656
O28 K6 O25 132.7(3) 7_565 5_656
O28 K6 O25 132.7(3) . 5_656
O20 K6 O25 116.5(3) . 5_656
O27 K6 U3 79.8(2) . .
O22 K6 U3 154.1(2) 3_656 .
O22 K6 U3 94.43(15) 5_656 .
O2 K6 U3 35.57(6) . .
O16 K6 U3 24.37(10) . .
O16 K6 U3 90.43(13) 7_565 .
O28 K6 U3 103.9(2) 7_565 .
O28 K6 U3 73.27(18) . .
O20 K6 U3 35.78(6) . .
O25 K6 U3 123.42(19) 5_656 .
O27 K6 U3 79.8(2) . 7_565
O22 K6 U3 94.43(15) 3_656 7_565
O22 K6 U3 154.11(19) 5_656 7_565
O2 K6 U3 35.57(6) . 7_565
O16 K6 U3 90.43(13) . 7_565
O16 K6 U3 24.37(10) 7_565 7_565
O28 K6 U3 73.27(18) 7_565 7_565
O28 K6 U3 103.9(2) . 7_565
O20 K6 U3 35.78(6) . 7_565
O25 K6 U3 123.42(19) 5_656 7_565
U3 K6 U3 66.12(6) . 7_565
O23 K7 O28 82.6(5) 6_556 2_554
O23 K7 O29 78.4(5) 6_556 .
O28 K7 O29 153.9(4) 2_554 .
O23 K7 O23A 114.1(5) 6_556 .
O28 K7 O23A 81.0(3) 2_554 .
O29 K7 O23A 123.1(4) . .
O23 K7 O28A 63.9(5) 6_556 2_554
O28 K7 O28A 28.4(3) 2_554 2_554
O29 K7 O28A 142.1(4) . 2_554
O23A K7 O28A 72.6(3) . 2_554
O23 K7 O22 129.5(5) 6_556 .
O28 K7 O22 132.8(3) 2_554 .
O29 K7 O22 73.3(3) . .
O23A K7 O22 55.9(3) . .
O28A K7 O22 127.9(3) 2_554 .
O23 K7 O23A 10.7(5) 6_556 6_556
O28 K7 O23A 93.3(3) 2_554 6_556
O29 K7 O23A 68.4(3) . 6_556
O23A K7 O23A 115.5(4) . 6_556
O28A K7 O23A 73.7(3) 2_554 6_556
O22 K7 O23A 120.6(3) . 6_556
O23 K7 K7 119.2(4) 6_556 7
O28 K7 K7 86.6(2) 2_554 7
O29 K7 K7 87.2(2) . 7
O23A K7 K7 122.9(3) . 7
O28A K7 K7 114.1(2) 2_554 7
O22 K7 K7 100.38(17) . 7
O23A K7 K7 120.7(2) 6_556 7
O23 K7 O23 126.5(6) 6_556 .
O28 K7 O23 85.8(4) 2_554 .
O29 K7 O23 119.9(4) . .
O23A K7 O23 12.6(3) . .
O28A K7 O23 82.3(4) 2_554 .
O22 K7 O23 48.1(4) . .
O23A K7 O23 127.2(4) 6_556 .
K7 K7 O23 112.0(4) 7 .
O23 K7 O25 125.7(5) 6_556 .
O28 K7 O25 144.2(3) 2_554 .
O29 K7 O25 47.7(3) . .
O23A K7 O25 102.1(3) . .
O28A K7 O25 170.3(4) 2_554 .
O22 K7 O25 48.7(2) . .
O23A K7 O25 116.0(3) 6_556 .
K7 K7 O25 61.45(14) 7 .
O23 K7 O25 91.4(4) . .
O23 K7 K6 65.4(5) 6_556 2_554
O28 K7 K6 38.6(2) 2_554 2_554
O29 K7 K6 116.0(3) . 2_554
O23A K7 K6 119.5(2) . 2_554
O28A K7 K6 52.5(2) 2_554 2_554
O22 K7 K6 164.9(3) . 2_554
O23A K7 K6 74.5(2) 6_556 2_554
K7 K7 K6 69.42(8) 7 2_554
O23 K7 K6 124.1(4) . 2_554
O25 K7 K6 127.66(19) . 2_554
O20 O2 U3 71.36(17) . 7_565
O20 O2 U3 71.36(17) . .
U3 O2 U3 137.1(3) 7_565 .
O20 O2 K6 80.6(4) . .
U3 O2 K6 97.10(19) 7_565 .
U3 O2 K6 97.10(19) . .
O17 O3 U3 72.8(3) . .
O17 O3 U2 71.8(3) . .
U3 O3 U2 128.9(2) . .
O17 O3 K5 174.5(4) . 5_656
U3 O3 K5 110.87(18) . 5_656
U2 O3 K5 107.62(17) . 5_656
O17 O3 K5 63.2(3) . .
U3 O3 K5 90.12(15) . .
U2 O3 K5 105.13(18) . .
K5 O3 K5 112.24(15) 5_656 .
U1 O4 K4 105.12(17) . 7_565
U1 O4 K4 105.12(17) . .
K4 O4 K4 127.5(3) 7_565 .
U3 O5 K1 110.4(2) . .
U3 O5 K3 129.7(2) . .
K1 O5 K3 82.09(14) . .
U3 O5 K2 122.4(2) . .
K1 O5 K2 102.51(16) . .
K3 O5 K2 99.95(16) . .
O7 O6 U1 71.5(3) . .
O7 O6 U2 72.6(3) . .
U1 O6 U2 129.3(2) . .
O7 O6 K4 126.0(3) . .
U1 O6 K4 90.48(15) . .
U2 O6 K4 139.94(19) . .
O6 O7 U1 71.6(3) . .
O6 O7 U2 70.8(3) . .
U1 O7 U2 128.2(2) . .
C2 O8 U3 122.2(4) 5_556 .
C2 O8 K5 114.7(4) 5_556 5_656
U3 O8 K5 122.6(2) . 5_656
C5 O9 U2 121.6(5) . .
C5 O9 K4 115.5(6) . 6_556
U2 O9 K4 94.56(17) . 6_556
U1 O10 K1 117.9(3) . .
U1 O10 K4 105.37(18) . 6_556
K1 O10 K4 107.82(16) . 6_556
U1 O10 K4 105.37(18) . 4_455
K1 O10 K4 107.82(16) . 4_455
K4 O10 K4 112.7(2) 6_556 4_455
C1 O11 K2 114.6(5) . .
C1 O11 K5 126.4(5) . 5_656
K2 O11 K5 92.39(16) . 5_656
U2 O12 K1 116.2(2) . .
U2 O12 K2 115.8(2) . .
K1 O12 K2 105.26(17) . .
U2 O12 K4 108.6(2) . 6_556
K1 O12 K4 108.52(16) . 6_556
K2 O12 K4 101.31(16) . 6_556
C1 O13 U3 122.6(5) 5_556 .
C3 O14 U1 120.9(4) . .
C3 O14 K4 105.9(4) . 6_556
U1 O14 K4 98.37(16) . 6_556
C3 O14 K4 119.8(4) . .
U1 O14 K4 88.21(16) . .
K4 O14 K4 121.50(17) 6_556 .
C2 O15 K2 118.7(5) . .
U3 O16 K5 110.0(2) . .
U3 O16 K6 112.0(2) . .
K5 O16 K6 93.67(16) . .
O3 O17 U2 71.2(3) . .
O3 O17 U3 70.3(3) . .
U2 O17 U3 126.8(2) . .
O3 O17 K5 88.9(3) . .
U2 O17 K5 116.26(19) . .
U3 O17 K5 98.25(17) . .
O3 O17 K1 117.5(3) . .
U2 O17 K1 85.73(15) . .
U3 O17 K1 80.87(14) . .
K5 O17 K1 150.89(17) . .
K3 O18 K5 134.2(2) . 1_455
C4 O19 U2 121.2(5) . .
C4 O19 K5 110.1(5) . 5_656
U2 O19 K5 120.1(2) . 5_656
C4 O19 K2 114.4(5) . .
U2 O19 K2 92.92(17) . .
K5 O19 K2 92.25(16) 5_656 .
O2 O20 U3 71.43(18) . 7_565
O2 O20 U3 71.43(18) . .
U3 O20 U3 137.2(3) 7_565 .
O2 O20 K1 115.2(5) . .
U3 O20 K1 88.55(19) 7_565 .
U3 O20 K1 88.55(19) . .
O2 O20 K6 70.9(4) . .
U3 O20 K6 93.66(18) 7_565 .
U3 O20 K6 93.66(18) . .
K1 O20 K6 173.9(3) . .
C3 O21 K2 129.8(5) . 6_656
C3 O21 K3 121.4(5) . 6_656
K2 O21 K3 108.54(18) 6_656 6_656
C3 O21 K1 88.2(4) . 6_656
K2 O21 K1 99.43(18) 6_656 6_656
K3 O21 K1 75.96(15) 6_656 6_656
C4 O22 K6 126.5(7) . 5_656
C4 O22 K7 104.3(7) . .
K6 O22 K7 116.7(3) 5_656 .
C4 O22 K5 82.0(6) . 5_656
K6 O22 K5 86.9(2) 5_656 5_656
K7 O22 K5 140.2(3) . 5_656
O23A O23 C5 72.0(17) . .
O23A O23 K7 132.0(19) . 6_656
C5 O23 K7 143.7(14) . 6_656
O23A O23 K7 54.9(15) . .
C5 O23 K7 94.1(11) . .
K7 O23 K7 121.7(6) 6_656 .
O23 O23A C5 71.7(17) . .
O23 O23A K7 112.5(17) . .
C5 O23A K7 113.7(7) . .
O23 O23A K7 37.3(16) . 6_656
C5 O23A K7 103.8(9) . 6_656
K7 O23A K7 115.8(4) . 6_656
K6 O25 K7 101.6(3) 5_656 7
K6 O25 K7 101.6(3) 5_656 .
K7 O25 K7 57.1(3) 7 .
K4 O26 K2 109.8(2) . 1_655
K6 O27 K5 92.0(2) . 7_565
K6 O27 K5 92.0(2) . .
K5 O27 K5 171.2(4) 7_565 .
O28A O28 K7 88.6(6) . 2
O28A O28 K6 105.2(6) . .
K7 O28 K6 107.7(3) 2 .
O28 O28A K7 63.0(5) . 2
K4 O30 K2 103.3(3) . 6_656
O11 C1 O13 125.5(7) . 5_556
O11 C1 C2 121.5(7) . .
O13 C1 C2 113.0(6) 5_556 .
O11 C1 K2 46.5(4) . .
O13 C1 K2 158.6(5) 5_556 .
C2 C1 K2 78.7(4) . .
O15 C2 O8 126.8(7) . 5_556
O15 C2 C1 117.9(7) . .
O8 C2 C1 115.3(6) 5_556 .
O15 C2 K2 43.1(4) . .
O8 C2 K2 166.3(5) 5_556 .
C1 C2 K2 75.5(4) . .
O15 C2 K5 80.7(4) . 1_455
O8 C2 K5 46.1(3) 5_556 1_455
C1 C2 K5 161.4(5) . 1_455
K2 C2 K5 122.9(2) . 1_455
O21 C3 O14 126.2(7) . .
O21 C3 C3 118.4(4) . 7_565
O14 C3 C3 115.5(4) . 7_565
O21 C3 K1 70.1(4) . 6_656
O14 C3 K1 123.9(5) . 6_656
C3 C3 K1 76.58(12) 7_565 6_656
O21 C3 K4 96.5(5) . 6_556
O14 C3 K4 53.1(4) . 6_556
C3 C3 K4 122.06(12) 7_565 6_556
K1 C3 K4 161.2(2) 6_656 6_556
O22 C4 O19 125.4(9) . .
O22 C4 C5 119.5(9) . .
O19 C4 C5 115.0(7) . .
O22 C4 K5 77.0(6) . 5_656
O19 C4 K5 49.2(4) . 5_656
C5 C4 K5 161.5(6) . 5_656
O23 C5 O23A 36.3(9) . .
O23 C5 O9 127.9(12) . .
O23A C5 O9 124.1(9) . .
O23 C5 C4 111.0(11) . .
O23A C5 C4 121.6(9) . .
O9 C5 C4 113.4(8) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O4 1.796(7) .
U1 O10 1.797(7) .
U1 O7 2.335(5) 7_565
U1 O7 2.335(5) .
U1 O6 2.336(5) 7_565
U1 O6 2.336(5) .
U1 O14 2.405(5) .
U1 O14 2.405(5) 7_565
U2 O1 1.778(5) .
U2 O12 1.798(5) .
U2 O6 2.341(5) .
U2 O3 2.344(5) .
U2 O17 2.352(5) .
U2 O7 2.366(5) .
U2 O19 2.392(5) .
U2 O9 2.434(5) .
U3 O16 1.785(5) .
U3 O5 1.800(5) .
U3 O3 2.331(5) .
U3 O20 2.351(3) .
U3 O2 2.351(3) .
U3 O17 2.365(5) .
U3 O13 2.385(5) .
U3 O8 2.397(5) .
K1 O10 2.681(7) .
K1 O5 2.753(5) .
K1 O5 2.753(5) 7_565
K1 O12 2.804(5) 7_565
K1 O12 2.804(5) .
K1 O20 3.016(8) .
K1 O21 3.155(6) 6_556
K1 O21 3.155(6) 4_455
K1 O17 3.344(5) 7_565
K1 O17 3.344(5) .
K1 C3 3.353(8) 6_556
K1 C3 3.353(8) 4_455
K2 O21 2.710(5) 6_556
K2 O15 2.719(6) .
K2 O11 2.752(5) .
K2 O12 2.838(5) .
K2 O26 2.901(7) 1_455
K2 O30 2.940(8) 6_556
K2 O5 2.993(5) .
K2 O19 3.044(6) .
K3 O18 2.677(6) .
K3 O18 2.677(6) 7_565
K3 O21 2.786(6) 6_556
K3 O21 2.786(6) 4_455
K3 O5 2.832(5) 7_565
K3 O5 2.832(5) .
K3 O24 2.844(9) .
K4 O26 2.781(7) .
K4 O30 2.816(8) .
K4 O14 2.879(5) 6_656
K4 O4 2.916(4) .
K4 O9 2.936(6) 6_656
K4 O6 2.981(5) .
K4 O12 3.001(5) 6_656
K4 O14 3.022(5) .
K4 O10 3.141(4) 6_656
K5 O19 2.754(5) 5_656
K5 O8 2.775(5) 5_656
K5 O17 2.830(5) .
K5 O18 2.883(6) 1_655
K5 O16 2.956(5) .
K5 O11 3.040(6) 5_656
K5 O27 3.138(2) .
K5 O3 3.154(5) 5_656
K5 O3 3.171(5) .
K5 O22 3.360(8) 5_656
K6 O27 2.883(12) .
K6 O22 2.922(9) 3_656
K6 O22 2.922(9) 5_656
K6 O2 2.973(9) .
K6 O16 2.986(5) .
K6 O16 2.986(5) 7_565
K6 O28 3.050(10) 7_565
K6 O28 3.050(10) .
K6 O20 3.104(8) .
K6 O25 3.217(12) 5_656
K7 O23 2.57(2) 6_556
K7 O28 2.717(10) 2_554
K7 O29 2.730(11) .
K7 O23A 2.958(12) .
K7 O28A 3.047(11) 2_554
K7 O22 3.129(10) .
K7 O23A 3.150(14) 6_556
K7 O23 3.34(2) .
K7 O25 3.428(12) .
O2 O20 1.500(10) .
O2 U3 2.351(3) 7_565
O3 O17 1.488(6) .
O3 K5 3.154(5) 5_656
O4 K4 2.916(4) 7_565
O6 O7 1.477(6) .
O8 C2 1.265(9) 5_556
O8 K5 2.775(5) 5_656
O9 C5 1.289(10) .
O9 K4 2.936(6) 6_556
O10 K4 3.141(4) 6_556
O10 K4 3.141(4) 4_455
O11 C1 1.226(9) .
O11 K5 3.040(6) 5_656
O12 K4 3.001(5) 6_556
O13 C1 1.301(9) 5_556
O14 C3 1.286(8) .
O14 K4 2.879(5) 6_556
O15 C2 1.243(8) .
O18 K5 2.883(6) 1_455
O19 C4 1.282(10) .
O19 K5 2.754(5) 5_656
O20 U3 2.351(3) 7_565
O21 C3 1.241(8) .
O21 K2 2.710(5) 6_656
O21 K3 2.786(6) 6_656
O21 K1 3.155(6) 6_656
O22 C4 1.237(10) .
O22 K6 2.922(9) 5_656
O22 K5 3.360(8) 5_656
O23 O23A 0.788(18) .
O23 C5 1.264(19) .
O23 K7 2.57(2) 6_656
O23A C5 1.265(13) .
O23A K7 3.150(14) 6_656
O25 K6 3.217(12) 5_656
O25 K7 3.428(12) 7
O26 K2 2.901(7) 1_655
O27 K5 3.138(2) 7_565
O28 O28A 1.448(13) .
O28 K7 2.717(10) 2
O28A K7 3.047(11) 2
O30 K2 2.940(8) 6_656
C1 O13 1.301(9) 5_556
C1 C2 1.551(10) .
C2 O8 1.265(9) 5_556
C3 C3 1.557(14) 7_565
C4 C5 1.555(13) .
